7. Rubbing It In
7.1 Phase Diagram and the Structure of Carbon Steel
7.1.1 Experimental Evaluation of Structures and Relation to Phase Diagram
|Looking at Structures|
|In the preceding chapters you learned a lot about phase diagrams. No let's apply
that to steel. Let's see what we can learn about the general structure of steel from the phase
diagram and from other resources.
How do we assess the structure of steel? Or of any other material? Well, you need to look at it. In chapter 4.1.1 we already looked at steel - with a transmission electron microscope at very high magnifications (> 10.000.000) and we saw a few of its atoms. They had a size of about 0.2 nm or 200 picometer (pm) and if you like, you can now impress your girl friend (your wife is probably not any more impressed by anything you do or say) by stating that you, personally, know about the pico structure of steel, something way better than just the ubiquitious nano everybody talks about.
But beware! You can't impress me or my buddies. We know that at very high magnification all crystals look pretty much the same. It's just like looking at, for example, this major piece of art at high magnification. Whatever part you look at, it looks pretty much like the pictures shown here. You really miss something by looking too closely!
Same thing for steel. Looking at its atoms is fun when you do it for the first time but quickly becomes boring. All atoms are rather alike after all; if you have seen one, you have seen them all. So now we take steels samples and look at their (comparatively coarse) micro structure with an optical microscope at magnifications not exceeding 1000-fold. That was the best one could do up to about 1960, and it is still the first thing you do when you want to find out about the structure of steel.
|Anything smaller than about 1 µm (or about 4.000 atoms in a row) is invisible in an optical microscope. But never fear, enough structural details are visible to make your mind boggle - provided we first prepare the specimen for the examination.|
|For that we first polish
the specimen to a high sheen. This can be done in several ways and the results may look the
same to the naked eye - but not to the microscope! You can, for example, achieve a nice shiny
surface by just holding your specimen against a rotating brush for a while. Easy - but useless
for structural investigations |
Polishing properly for structural investigations is not all that easy. This is why I decided to give you an extra module for this topic.
After perfect polishing we have a perfectly flat and structureless surface that just terminates the crystal without producing any damage of its own in surface near layers. You can now look at it with your optical microscope and what you will see is exactly nothing . That's the meaning of the word "structureless".
|Now we need to invoke a bit of black art. We concoct
called a defect etchant, that has certain magical properties.
For example, if you drink it during a full moon at midnight in a cemetery, you will be dead.
It even works if there is no full moon, everywhere and at any hour! Defect etchants are typically
rather aggressive so don't fool around with defect etching if you don't know exactly what
you are doing. |
Let's not drink it but apply it to our polished steel (after we cleaned the polished surface in more or less tricky ways). If your "etchant " (for short) for carbon steel was cooked up the right way, and you immerse your polished sample in it, it will now do the following:
|Schematically, this is what happens|
|In reality you might see something like this:|
|The black stuff is cementite; grain boundaries are not really visible here. The cementite shows a kind of "zebra" structure (I'll come to that soon). If the lamellae in that structure would be a little bit smaller, the light microscope couldn't resolve the structure anymore. What you see then looks like this:|
we have scanning electron microscopes
(SEM) that allow to look at surfaces with a resolution far better than that of a light microscope.
They are also far more expensive than a light microscope and it is more time consuming to
This is what you might see in a case where you wouldn't see much in a light microscope:
|The two examples already show that structure etching (also called defect etching) is an extremely powerful technique! Generations of Materials Scientists (then also called Metallographers ) relied on it and most of our empirical knowledge base about steel and pretty much all other metals, semiconductors and ceramics comes from structure etching.|
However, you only see the structure that the etchant was designed to reveal. What will happen
if you use the etchant that produced the pictures above for "carbon steel" when
you use it for phosphorous steel?
Or for stainless steel? Or...? There is no guarantee that some "carbon steel" etchant
works for these materials too. |
You get it: there is work to be done.
Every material requires its own etchant. Since there are no simple guidelines for concocting
these potions, and since tiny details matter a lot, defect etching still counts among the
black arts in modern science. Of course, after long years of applying it to iron and steel,
the art of brewing and applying the various concoctions for steel are now taught in undergraduate
classes at Hogwarts and at all Materials Science and Engineering
Institutes. But it is still very advanced magic to come up with a new brew for some new kind
material. Take gallium nitride (GaN) as an example for a material that became very important
recently (look it up!). There is not yet a good defect etchant out there. |
The science module gives you details about defect etching of steel.
|What I just did was to give you an idea that when you stare into your microscope,
most of the difficult work has already been done. Every
|In chapter 3 we have tortured steel and innocent bystanders by pulling them up to the breaking point. Now let's look at what has happened to the microstructure of the specimens sentenced to a tensile tests. We want to know how the microstructure changes during the various phases of plastic deformation and fracture. This is going to be real work!|
|We have specimens from several types of steel and we need to look at their structure before we did the tensile test and after we elongated them plastically just a little bit, a bit more, up to a lot . We should look at the pieces after they fractured, and on elongated specimens after we heated them for a while at some temperature, including the process called normalizing, and so on.|
|Each time we have to cut a sample, grind and
polish it, etch it, look at it, take pictures and discuss them. Not a big deal scientifically
- but a lot of work. |
You should certainly do that yourself for a while. It's the only way to get a feeling for what can be done. But when you become a Professor, it is better to train a lab technician for the job. He (and especially she) will be far better (and cheaper) than you at doing this kind of work.
Going through the program above she will also produce far more pictures than I can include here. It is also not much fun to go through umpteenth pictures, discussing every one at length. You know this if you have ever been the target of a slide show by a well meaning relative.
|It's also a lot of work to find out what kind of structural changes occur between high and low temperatures for a given piece of steel from only evaluating all these pictures. So let's invoke our central science dogma. Since there is nothing more practical than a good theory, let's first look at the phase diagram and see if we can deduce what we should see. If we can do this with confidence, we don't need to look at too many pictures. Same thing for deformation experiments. If you know the theory, you only need to analyze a few relevant samples to get you oriented.|
|Below is the relevant part of the iron-carbon phase diagram around the especially important eutectoid composition. Let's see if we can predict what kind of structure we will get, taking into account that the crystal will never make it to nirvana proper. Why? Because for nirvana we know the structure: Just perfect big crystals of whatever phases we need.|
|First, we look at a steel with the so-called eutectoid composition, meaning
the composition at about 0,7 wt % carbon. That's where the g phase can change into the mixed a+ cementite phase directly, without having to go through
the a + g or g
+ Fe3C region. This is indicated by the green line. |
This is exactly the same thing that we found for the case of an eutectic composition not so long ago - except that the phase change here is not from liquid to solid but from solid to solid. That's why we call it eutectoid instead of eutectic, just as you might call (insert politician or banker of your choice) humanoid (= similar to humans) instead of human. While we are at it, here are two more "oids":
|Steel with less than 0,7 % carbon we call hypoeutectoid. Should there be more than 0,7 % carbon, the steel is hyper eutectoid.|
|Sorry for throwing Greek at you once more, but in
this case it's easy: |
"Hypo" means "below" or "under" as in "hypodermic", under the skin.
"Hyper" means "above" or "excessive", as in "hyperactive ".
OK - once more so you get it: (">" and "<" mean "larger as" or "smaller as", respectively):
|Yes, I could have used everyday words like "proper", "low" and "high" instead of "eutectoid", "hypoeutectoid" and "hypereutectoid" carbon steels, respectively. But if you want to be a member of the gang you must learn its slang.|
|If we have the eutectoid composition and hold it above the transition temperature around 1000 K (727 oC, 1341 oF), we will find the g structure called austenite. At this temperature we also have enough mobile vacancies to allow some motion or diffusion of the atoms. Our steel will then happily work on changing the microstructure of the austenite to a nirvana structure. It will not succeed in finite times but getting close.|
|If we allow it some time,
we could reasonably expect that its structure will consist of big grains of the pure g-phase or austenite, and that it
will be rather free of dislocations or other big defects. |
I'd love to show you a picture of this serene state of being, but it's rather hard to look at red-hot things close-up with a microscope. It is actually impossible. We could get a picture with tricky and expensive equipment involving X-rays and so on, but why should we bother? Why should we spend a lot of (your) money and (our) time to show that things really are what they simply must be? Behold the wisdom of the central dogma!
|The best I can
do is to show you a picture of the austenite structure as we find it in some alloy steels ("stainless steel" or "austenitic
steel" variants) at room temperature. If you add substantial amounts of
alloy elements like nickel (Ni) and chromium (Cr) to the iron-carbon mix, the transition temperature for
the austenite ® ferrite + Fe3C phase transition goes
down to values where it cannot take place anymore (too cold to move). Austenite then exists
at room temperature as a metastable phase. We cannot expect it, however, to be as perfect as the real thing
at those low temperatures. |
Nevertheless, here goes. The following picture shows what a rather perfect austenite structure looks like under a light optical microscope at low magnification:
|This could be austenitic stainless steel from your kitchen sink. It looks polished because it is polished and thus would show no structure under the microscope. We know already why we see something here.|
|Once more we see the structure after defect etching. As stated above, in order to render the bigger defects visible, we need to etch our specimen after we polished it to a high sheen. Grain boundaries then typically produce tiny grooves and steps that appear as the black lines in the optical micrograph above.|
that I could easily cheat on you. I would never do that, of course, but what you see above
could just as well be a picture of the microstructure of copper (Cu), gold, (Au), aluminum
(Al), silicon (Si),..., whatever. There is no way of telling just by looking at the picture.
But you know that Materials Scientists and Engineers don't cheat people out of their money
since you rarely see them driving Lamborghinis or Porsches. So you can trust us in science
matters, too. |
If you're now inclined to send me (large) amounts of money, I will happily invest it for you.
|So defect etching does help you to see at lot of
structure on the surface - but beware! You will not see everything. With a light optical microscope
you cannot see small "nano" things at all, even it they are properly etched. Then
other structures might be there but might not have been revealed by the etchant. And beware
of the bane of all metallographers: artifacts! Things
that are not there but nevertheless show up. |
Defect etching was and is crucial not only for iron and steel but also, for example, in silicon technology. The link takes you deep into defect etching in silicon, the probably most thoroughly investigated material in this respect.
| Be that as it may, what we see in the picture above is pretty much what we would
have expected: We see a nice poly crystal with irregular and rather large grains. Grain sizes
around 40 µm - roughly the thickness of a hair - are
considered large |
Nothing spectacular otherwise. The faint structure in the background may have some significance but it also could be an artifact.
Nevertheless, the fact that we can see a good part of the structure of austenitic fcc steel (or other materials) after some defect etching is of utmost importance: it started Materials Science!
|Before about the middle of the 19th century, working
with iron and steel was a purely empiric enterprise, based on experience and not much else.
With the advent of microscopy, the science and technology of materials like steel started.
Researchers then had only optical microscopes to look at the microstructures of things (and no quantum theory, statistical thermodynamics and other basic tools).
Electron microscopes hadn't been invented (that had to wait until around 1960), not to mention high-resolution electron microscopes (HRTEM), that allow to see crystal structures or atom columns directly, which were not available before 1975.
|Come to think of
it, even atoms hadn't been "invented" yet
in the 19th century. Ludwig Boltzmann,
one of the most outspoken proponents of "atoms" as something real, was ridiculed
as late as the turn of the century (1900) not only by Wilhelm Ostwald
(of "Ostwald ripening"
fame; I'll get to that) and Ernst Mach
(of supersonic velocity fame) but also by no less a celebrity than Max
Planck, who opened the door to quantum theory but had a hard time to believe in the
existence of atoms. |
It was Albert Einstein in 1905 who put an end to that and firmly established atoms as being not only real physical entities but the only entities that exist besides photons (which, incidentally, he introduced at the same time).
|Now I have a question for you: Did atoms (or about anything else in science) get "invented" or "discovered "? Are they just figments of human thinking; social constructs that will be laughed at by scientists in the future, or are they real entities, existing independent of humans at all times? This link will tell.|
|Without knowing about atoms you can't fully understand crystals. Without crystals you can't have crystal defects. Without crystal defects you can't describe the microstructure of materials.
Not knowing the microstructure of materials prevents you from understanding
most of their properties. |
It doesn't prevent you from describing them, however. For example, by just doing measurements you can correlate the carbon concentration and hardness and thus answer the "what" question. "What is carbon doing in iron"? "It makes it harder"! You can even do that quantitatively with numbers. What you cannot do is answering the "why" questions. "Why is carbon making steel harder"? "I don't know"!
|So you, the not-so-ancient smith in the 19th century (now called Engineer), will prepare specimens, etch them somehow, and put them under your microscope. If you do it right you are going to see things. Even if you don't have the faintest idea what it really is that you see, you can always describe it in words and measure parameters like size or distribution.|
|If you are among the first ones doing this, you are going to see things that nobody has seen before. If you miss proper words for describing what you see, you just invent some new ones like "pearlite", "cementite", "martensite" or "bainite" (not to mention "ledeburite"). You still don't know what it is but now can talk and write about it - it's not unlike politics at this stage.|
|In what follows we look at optical "micrographs" like our early steel scientists and, while we are not going to see atoms, small precipitates, dislocations and the like, I promise that what we are going to see will be quite enough to make your head spin. In other words: we are looking at parts of the microstructure of iron / steel. For the rest we would need to employ electron microscopy or other sophisticated techniques.|
|And in contrast to the pioneers of old we now know what we see! Well - make that: I know what we see, and I will tell you.|
© H. Föll (Iron, Steel and Swords script)